1 CRUSHING BRICK BLENDS FOR SUB-BASE APPLICATIONS Can recycled crushed brick blended with crushed concrete create effective subbase applications? And if so, do such applications meet statutory specifications? Thurairatnam Aatheesan and Arul Arulrajah discuss the science. Recycling and reuse of waste materials is a topic of global concern and of great international interest. The urgent need for recycling is driven mainly by environmental considerations, due to the increased scarcity of natural resources and the increasing cost of landfill in most countries. Construction and demolition (C&D) materials are generated by regeneration of infrastructure such as demolition activities and accounts for the major proportion of the waste materials present in landfills. Recycled crushed brick and crushed concrete are viable substitute materials for natural construction materials in engineering applications such as pavement sub-base and other road construction applications. Some countries have been using recycled C&D materials in civil engineering applications but there is still scope for wider engineering applications of such recycled materials. This paper primarily focuses on the applicability of crushed brick blends with crushed concrete in pavement sub-base material as well as bedding and backfill material for drainage systems. The engineering properties of crushed brick blended with crushed concrete were investigated by means of laboratory testing. A suite of laboratory tests was conducted on blend mixes of 10 per cent, 15 per cent, 20 per cent, 25 per cent and 30 per cent of crushed brick with crushed concrete. The resulting engineering properties were compared with the existing local authority specifications for flexible pavement sub-base and drainage material. EXISTING LOCAL SPECIFICATIONS Pavement sub-base VicRoads is a statutory authority responsible for managing the road network (roads and bridges) in Victoria, Australia. It classifies recycled crushed concrete for pavement subbase and light duty base as Class CC2, Class CC3 and Class CC4 (VicRoads, 2006). This classification is based on the physical and SIEVE SIZE AS (MM) TEST VALUE TARGET GRADING (% PASSING) mechanical properties of crushed concrete. Table 1 presents the physical properties of crushed concrete as specified by VicRoads. Table 2 presents the before compaction grading limits for 20mm Class CC3 crushed concrete. Table 3 presents the after compaction grading requirements for Class 3 crushed rock sub-base which is applicable for crushed concrete. TEST CLASS CC2 CLASS CC3 CLASS CC4 Liquid limit (%) (max) Plasticity index (max) California Bearing Ratio (%) (min) Los Angeles abrasion loss (max) Flakiness index Table 1: Physical properties of crushed concrete (VicRoads, 2007). LIMIT OF GRADING TEST VALUE BEFORE COMPACTION (% PASSING) Table 2: Grading requirement for 20mm Class CC3 crushed concrete (VicRoads, 2007). 14 Quarry July 2011
2 SPECIAL REPORT - RECYCLING Bedding and backfill material Melbourne Water is the authorised governing body for local drainage systems. Melbourne Water classifies backfill and bedding material as Grade A and Grade B material. Melbourne Water specification for the supply of crushed rock to their work sites is summarised in Tables 4 and Table 5 (Melbourne Water, 2001). ENGINEERING PROPERTIES OF CRUSHED BRICK BLENDS Samples of crushed brick and crushed concrete were collected from the Alex Fraser Group recycling site at Laverton North, Victoria, as well as the Delta Group recycling site at Sunshine, Victoria, Australia. Alex Fraser Group and Delta Group are the leading suppliers of high-quality sustainable civil construction materials in Australia, supplying recycled materials such as crushed brick, crushed concrete and crushed rock in various classes. The crushed brick and crushed concrete used in this research had a maximum aggregate size of 20mm. Laboratory tests were undertaken on blended mixtures of 10 per cent, 15 per cent, 20 per cent, 25 per cent and 30 per cent crushed brick with crushed concrete. The laboratory tests included modified compaction, particle density, water absorption, California Bearing Ratio (CBR), Los Angeles abrasion, Atterberg limit, ph, organic content, wet and dry strength and clay content. The blend mixtures were prepared by hand mixing to the required percentages by weight. Crushed brick from Alex Fraser Recycling site typically consists of 70 per cent brick and 30 per cent other materials such as asphalt, concrete and rock. Crushed brick from the Delta recycling site on the other hand typically comprises 40 per cent brick, 55 per cent crushed concrete and five per cent asphalt. The laboratory tests were performed in accordance with Australian Standards AS 1141 (1996) and AS 1289 (1998). Particle density and water absorption tests were performed in both coarse (retained on 4.75mm sieve) and fine (passing 4.75mm sieve) material. The physical characteristics of crushed brick blends with crushed concrete obtained from the laboratory tests are summarised in Table 6 (see page 16). The particle size distribution results prior to compaction and after compaction for crushed brick blended with crushed concrete (Class 3) is summarised in Tables 7 and Table 8 (see page 17). 70CC3 refers to 30 per cent crushed brick content blended with 70 per cent crushed concrete (CC3) by weight. Particle densities of coarse aggregates (retained on 4.75mm sieve) are higher than the fine aggregates (passing 4.75mm) and water absorptions of coarse aggregates are less than the fine aggregates. The coarse aggregates of blends may contain the natural aggregates used in concrete and the fine aggregates may contain cementitious mortar. This may lead to the higher particle density and lower water absorption in coarse aggregates and lower particle density and higher water absorption in finer aggregates. The ph values of all blends are over 7 and this indicates that the blends are alkaline by nature. TEST SIEVE METRIC AS COMPARISON WITH LOCAL SPECIFICATIONS Pavement sub-base The laboratory test results were subsequently compared with existing local specifications for pavement sub-base applications. The Los Angeles abrasion loss values are clearly within the maximum value of 35 normally adopted by VicRoads for Class 3 subbase pavement materials. The wet and dry strength results indicate that the mechanical properties of the crushed concrete blends do not vary significantly between the wet and dry states. This indicates that little breakdown is occurring in the coarse fraction of the blend from a dry to saturated surface dry condition. The wet and dry strength test indicates the durability of materials when they are in saturated surface dry condition and complete SIEVE SIZE (MM) GRADED CRUSHED ROCK Limits of percentage passing sieve aperture by mass Aperture 20mm B grade 20mm A grade 26.5mm mm mm mm mm mm mm mm mm mm Table 4: Grading limits for crushed rock (Melbourne Water, 2001). TEST VALUE Atterberg liquid limit Plasticity index (max) 16 4 Los Angeles abrasion loss Table 5: Other requirements for crushed rock (Melbourne Water, 2001). PERMITTED GRADING AFTER COMPACTION (% PASSING) NOMINAL SIZE 20MM Table 3: Grading requirements for Class 3 sub-base crushed rock after compaction (VicRoads, 1995). Quarry July
3 dry condition. Materials with wet and dry strength variations of less than 35 percent are considered durable (Lay, 1998). As the clay content in all the blends was low, the plastic limit and liquid limit could not be obtained. This is because the Atterberg limit is directly related to clay mineralogy and so higher clay contents result in higher plasticity. This aspect may mean that some difficulties may occur with the workability of the crushed concrete blends as cohesion of particles and a tight prepared surface is usually a sought after characteristic. A field trial of the crushed concrete would best determine the degree of difficulties that may be experienced. The addition of small quantities of clayey sand or plastic crusher fines may overcome this potential issue. The grading limits of all blends before compaction using 20mm Class CC3 crushed concrete were within VicRoads lower and upper bounds for Class CC3 crushed concrete sub-base application, as shown in Figure 1 (see page 17). The grading limits of all blends after compaction as compared with VicRoads requirements for Class 3 crushed rock sub-base in flexible pavement is shown in Figure 2 (see page 18). The grading limits of most blends were well within the upper bounds of the grading envelope. The after compaction grading curves show that some breakdown is occurring under compaction; however compliance with normal after compaction requirements is still achieved. The before and after compaction grading curves (ie degree of breakdown occurring during compaction) would suggest that a maximum of 15 per cent crushed brick should be added to a Class 3 crushed concrete sub-base in order to maintain an acceptable after compaction grading. It is likely that the breakdown is occurring in both the crushed brick and the crushed concrete components. The materials appear to be remaining reasonably well graded through the compaction process and this will generally aid the compaction process. Figure 3 presents the CBR results for the crushed brick blends (see page 18). The CBR values of the tested blends were above 80 per cent and found to satisfy the VicRoads requirement for Class CC3 material. The differences in CBR results for the Series 1 and Series 2 tests could be due to slight differences in the aggregate strengths and proportions since they were carried out on different bulk samples and several months apart. SAMPLE DESCRIPTION 70CC3 75CC3 80CC3 85CC3 90CC3 100CC3 Brick content (%) by weight Material source AFR DR AFR DR AFR AFR AFR AFR Test description Test results Particle density (Coarse) (t/m 3 ) - Series Particle density (Coarse) (t/m 3 ) - Series Particle density (Fine) (t/m 3 ) Water absorption (Coarse) (%) - Series Water absorption (Coarse) (%) - Series Water absorption (Fine) (%) CBR (%) Series Series Los Angeles abrasion ph Compaction (modified) Wet and dry strength (kn) Atterberg limit Max dry density (t/m 3 ) Opt moisture content (%) Wet Dry Strength variation (%) Plastic limit NO NO NO NO NO NO Liquid limit NO NO NO NO NO NO Plasticity Index NP NP NP NP NP NP Clay content (%) Note: AFR Alex Fraser Recycling; DR Delta Recycling 70CC3 refers to 30 per cent crushed brick content blended with 70 per cent crushed concrete (CC3) by weight. NO Not obtainable. NP Non-plastic. Table 6: Engineering properties of crushed brick blended with crushed concrete (Class 3). 16 Quarry July 2011
4 SPECIAL REPORT - RECYCLING Bedding and backfill material The laboratory test results were also compared with local specifications for bedding and backfill material. The grading curves of all blends as compared with Melbourne Water specifications for Grades A and B materials are presented in Figures 4 and 5 respectively (see page 18). The grading limits of all blends for Grades A and B bedding and backfill material were found to be within the Melbourne Water specified lower and upper bounds. However, some finer particles for Grade B materials were found to be on the limit. The tests results of the crushed brick blends satisfied all Melbourne Water requirements for both Grades A and B materials except the Los Angeles requirements for Grade A material which were found to be on the limit. CONCLUSIONS AND RECOMMENDATIONS The results of the laboratory testing undertaken in this research has shown overall that the incorporation of crushed brick into crushed concrete has low to minimal effect on the physical and mechanical properties of the original material. Therefore, the crushed brick blends with crushed concrete were demonstrated to satisfactorily meet the current VicRoads specification requirements. The research indicates that initially up to 15 per cent crushed brick could be safely added to Class 3 crushed concrete blends. The degree of breakdown occurring in the crushed brick blend is on the limit of what would be acceptable for this material. Depending on the results of field trials, it may be possible to increase the percentage of crushed brick added in the future. The grading limits of all crushed brick blends, before and after compaction were also within VicRoads specified upper and lower bounds for crushed concrete (CC3) while some grading for the crushed brick blends were close to the specified limits. The wet and dry strength variation tests showed low variations (less than 10 per cent) for a number of blends. This indicates that there is little deterioration in strength from a dry to a saturated condition. The grading limits of all crushed brick blends with up to 30 per cent crushed brick content were found to be within Melbourne Water upper and lower bound grading curves for Grade A and Grade B backfill and bedding material. The crushed brick blends satisfied all Melbourne Water requirements SAMPLE DESCRIPTION 70CC3 75CC3 80CC3 85CC3 90CC3 100CC3 Brick content (%) by weight Particle size (mm) Percentage of total passing (%) Table 7: Particle size distribution (before compaction). SAMPLE DESCRIPTION 70CC3 75CC3 80CC3 85CC3 90CC3 100CC3 Brick content (%) by weight Particle size (mm) Percentage of total passing (%) Table 8: Particle size distribution (after compaction). Figure 1: Particle size distribution (before compaction) of crushed brick blends. Quarry July
5 for both Grade A and Grade B materials except the Los Angeles Abrasion requirements for Grade A material, where further testing of different blends is recommended. This paper was written by the following contributors: Aatheesan T, Swinburne University of Technology, Melbourne, Australia. Arulrajah A, Swinburne University of Technology, Melbourne, Australia. Newman G, VicRoads, Melbourne, Australia. Bo MW, DST Consulting Engineers, Ontario, Canada. Wilson J, Swinburne University of Technology, Melbourne, Australia. Figure 2: Particle size distribution (after compaction) of crushed brick blends. Figure 3: California Bearing Ratio of crushed brick blends. Figure 4: Particle size distribution of crushed brick blends for bedding and backfill materials (Grade A). ACKNOWLEDGEMENTS This paper was originally printed in Australian Geomechanics, Volume 44, No 2, June 2009, and is reprinted in Quarry with kind permission. The authors acknowledge Sustainability Victoria for funding this research project (Contract No: 3887) and acknowledge Alex Fraser Group and Delta Group for providing samples of crushed brick and crushed concrete as well as their technical assistance on this project. The authors thank VicRoads for permission to publish this paper. The views expressed are those of the authors and do not necessarily represent those of VicRoads. ABOUT CENTRE FOR SUSTAINABLE RESEARCH, SWINBURNE Civil infrastructure research at Swinburne University of Technology is undertaken within the Centre for Sustainable Infrastructure, commonly known as CSI-Swinburne. CSI provides a focus for multi-disciplinary research in the field of sustainable civil infrastructure, which is a topic of national importance in the 21st century, and will expand research links through collaboration both nationally and internationally in a manner consistent with the Federal Government s research model of hubs and spokes. CSI has three major research programs consisting of a series of projects involving industry partners, centre staff, research fellows and graduate students. The three research program areas are as follows: Advanced Structural and Geotechnical Systems (ASGS), Transportation Systems (TS) and Water Resources Modelling (WRM). Swinburne University is continuing its 18 Quarry July 2011
6 SPECIAL REPORT - RECYCLING Figure 5: Particle size distribution of crushed brick blends for bedding and backfill materials (Grade B). research focus on recycled materials with the potential to replace quarried products. Associate Professor Arul Arulrajah, Centre for Sustainable Research, Swinburne University of Technology, welcomes industry inquiries, REFERENCES Australian Standards AS1141 (1996). Method for sampling and testing aggregates. In: Standards Australia, Standards Association of Australia. Australian Standards AS1289 (1998). Method of testing soils for engineering purposes. In: Standards Australia, Standards Association of Australia. Melbourne Water. Sands crushed rock and crushed scoria. In: Specification 21.A.038, August Lay MG. Handbook of road technology (Third edition, Volume 1). Gordon and Breach, Netherlands, VicRoads (1995). Standard specifications for road works and bridge works. Section 304: Flexible pavement construction, February. VicRoads (2007). Standard specifications for road works and bridge works. Section 820: Recycled crushed concrete for pavement sub-base and light duty base.